Smoothing the single-crystal to single-crystal conversions of a two-dimensional metal-organic framework via the hetero-metal doping of the linear trimetallic secondary building unit.
Chao, Meng-Yao; Chen, Jing; Young, David J.; Zhang, Wen-Hua; Lang, Jian-Ping; Dalton transactions (Cambridge, England : 2003) 47 (2018) 13722–13729; doi:10.1039/c8dt02813c

data_7047515
_publ_section_title
;
 Smoothing the single-crystal to single-crystal conversions of a
 two-dimensional metal-organic framework via the hetero-metal doping of
 the linear trimetallic secondary building unit.
;
_journal_issue                   38
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              13722
_journal_page_last               13729
_journal_paper_doi               10.1039/c8dt02813c
_journal_volume                  47
_journal_year                    2018
_chemical_formula_moiety
'C27 H15 Cd1.13 Co0.38 O6, 2(C5 H11 N O) [+ solvent]'
_chemical_formula_sum            'C37 H37 Cd1.12 Co0.38 N2 O8'
_chemical_formula_weight         786.23
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2016/6
_audit_update_record
;
2018-07-09 deposited with the CCDC.
2018-09-10 downloaded from the CCDC.
;
_cell_angle_alpha                68.842(3)
_cell_angle_beta                 81.757(4)
_cell_angle_gamma                87.126(4)
_cell_formula_units_Z            2
_cell_length_a                   10.4753(7)
_cell_length_b                   14.5642(5)
_cell_length_c                   14.8464(5)
_cell_measurement_reflns_used    5224
_cell_measurement_temperature    213(2)
_cell_measurement_theta_max      25.6900
_cell_measurement_theta_min      3.1880
_cell_volume                     2090.52(18)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.32 (release 02-08-2013 CrysAlis171 .NET)
(compiled Aug  2 2013,16:46:58)
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.32 (release 02-08-2013 CrysAlis171 .NET)
(compiled Aug  2 2013,16:46:58)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.32 (release 02-08-2013 CrysAlis171 .NET)
(compiled Aug  2 2013,16:46:58)
;
_computing_molecular_graphics    'SHELXL-2013 (Sheldrick, 2013)'
_computing_publication_material  'publCIF (Westrip, 2010)'
_computing_structure_refinement  'SHELXL-2013 (Sheldrick, 2013)'
_computing_structure_solution    'SHELXL-2013 (Sheldrick, 2013)'
_diffrn_ambient_temperature      213(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.879
_diffrn_measurement_device_type  'Xcalibur, Atlas, Gemini'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0460
_diffrn_reflns_av_unetI/netI     0.0886
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.879
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            25516
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.879
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         30.904
_diffrn_reflns_theta_min         2.807
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    0.773
_exptl_absorpt_correction_T_max  0.927
_exptl_absorpt_correction_T_min  0.833
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.32 (release 02-08-2013 CrysAlis171 .NET)
(compiled Aug  2 2013,16:46:58)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            purple
_exptl_crystal_density_diffrn    1.249
_exptl_crystal_description       block
_exptl_crystal_F_000             802
_exptl_crystal_size_max          0.300
_exptl_crystal_size_mid          0.200
_exptl_crystal_size_min          0.100
_refine_diff_density_max         1.021
_refine_diff_density_min         -1.092
_refine_diff_density_rms         0.080
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.015
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     561
_refine_ls_number_reflns         11603
_refine_ls_number_restraints     446
_refine_ls_restrained_S_all      1.014
_refine_ls_R_factor_all          0.1221
_refine_ls_R_factor_gt           0.0608
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0761P)^2^+0.1701P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1449
_refine_ls_wR_factor_ref         0.1813
_reflns_Friedel_coverage         0.000
_reflns_number_gt                6225
_reflns_number_total             11603
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c8dt02813c2.cif
_cod_data_source_block           1a
_cod_depositor_comments
'Adding full bibliography for 7047515--7047518.cif.'
_cod_database_code               7047515
_shelx_shelxl_version_number     2016/6
_shelx_estimated_absorpt_t_min   0.801
_shelx_estimated_absorpt_t_max   0.927
_shelx_res_checksum              75497
_shelx_fab_checksum              18937